submitted in partial fulfillment of the requirements for the degree of
Author : Alberico Sabbadini
Student ID : 1591649
Supervisor : prof. dr. Martin van Hecke dr. Corentin Coulais
2ndcorrector : dr. Daniela Kraft
Hierarchically folding mechanical
metamaterials (of rank III)
Huygens-Kamerlingh Onnes Laboratory, Leiden University P.O. Box 9500, 2300 RA Leiden, The Netherlands
March 4, 2016
In recent years, a number of artificial materials (so called metamaterials) have been developed, tailoring exotic responses to mechanical stress by exploiting geometrical features. A particular
class of 2D metamaterials consists of tilings of polygons that can fold onto themselves by exploiting a mechanical instability triggered by compression. A subclass of these materials shows a sequence of two ordered states (one partially and one fully closed)
when biaxially compressed; however, the reason why such networks fold in multiple steps is yet elusive and we are unaware
of a general rule to design them; it is even unknown whether it is possible to increase the number of ordered states sequentially
reached by a network during the folding process. In order to answer these questions, first we investigate a variety of designs to
determine the role played by symmetries, topology and elastic energy; secondly, we focus on a hierarchical approach to design a
network with three folding stages; finally, we fully characterize the mechanical response of this new network and we study how
1 Introduction 1
1.1 Overview 1
1.2 Physics of the experiment 3
2 Experimental realization 11
2.1 Experimental apparatus 11
2.2 Exploration phase 18
2.3 Focus: the hierarchical approach 24
3 Results 29
3.1 Rank III folding 29
3.2 Rotations and symmetries 33
3.3 Order parameter 36
4 Conclusions 41
5 Appendix 1 45
Figure 1.1: Rotation of squares caused by uni-axial compression.
In the fast-paced technological evolution of our times, the demand for new materials is ever in-creasing; in this context, materials with easily tun-able properties can play a key role, and will likely do even more so in the near future.
A number of new researches [1–4] have thus emerged in the field of metamaterials, materials that exploit their geometries to gain novel proper-ties not found in nature[5,6].
A relevant example of such metamaterials is the so-called ”Holey Sheet” [3, 7] (shown in fig-ure 1.2a), a square-latticed array of circular holes drilled through an elastic polymer; under uni-axial compression, this material shows auxetic behaviour: when compressed along one axis, it shrinks also along the perpendicular direction (Poisson’s coefficent ν < 0). Looking at it from
a different point of view, this material can be thought to consist of square-shaped blocks connected via thin beams: when a compressing strain is applied, the thin beams bend and make the squares rotate (see figure1.1). The rotation ends when the squares reach full contact with each other, in a more compact configuration; in other words, the system effectively folds onto itself, closing the holes (as shown in figure1.2b).
(a) (b) (c)
Figure 1.2:a) A holey sheet. b) A folded holey sheet. c) A rank II network.
(shown in figure 1.2c) that exploits mechanical instabilities to fold twice (a more formal definition of folding process and folded state will be given in the next paragraph); this result was obtained by introducing a hierar-chyin the connecting beams, differentiating them into two sets that would deform at two separate stages. Despite this finding, however, it is still un-clear which features of the network determine its behaviour: what role is played by the connectivity of the individual squares? Are the symmetries (local or global) of any importance? So far, the behaviour of some particu-lar geometries is known empirically, but a predictive theory is still elusive, and it is generally impossible to determinea prioriwhether a network has ordered folded states or upon which conditions it can access them.
The goal of this master thesis project is to expand the understanding of these folding processes by means of further investigations on geometries with multiple folded states. In order to do so, at first we explored differ-ent ways of obtaining such systems. In a second stage of this project, we focused on extending the hierarchical approach used in , as it would provide insight on both multi-foldable networks in general, and on the specific subclass of hierarchical networks in particular. Finally, after suc-cessfully building a hierarchical network with three folded states, we char-acterized its mechanical and topological behaviour, and compared it with the behaviour of its predecessors.
1.2 Physics of the experiment 3
Physics of the experiment
Before we proceed with describing the mechanisms through which fold-ing processes take place, it makes sense to introduce a basic theoretical framework. Let us then start with some definitions:
Folding: A deformation process that leads to a total reduction in vol-ume due to closures of holes in the system.
Unit cell: A part of the network that, during the folding process, move without internal deformation. In the holey sheet, the individ-ual squares are the unit cells.
Self contact: Contact between parts of the network.
Folded state:An ordered configuration in which parts of the network have reached self contact, biaxial compression doesn’t lead directly to additional bending of the links, and the total volume is a fraction of that in the original state. In the final, fully folded state, all squares have reached self contact and form a square lattice.
Jammed state: A disordered configuration (i.e. the system doesn’t show any spatial symmetry) in which parts of the network have reached self contact and the system cannot be compressed further without deforming the squares.
Multiple folding (/multi-step folding): A folding process during which the system reaches a number of folded states between its open and its fully closed configurations.
Folding path:The sequence of deformations followed by the network during the folding process; it can also be viewed as the sequence of energy configurations of the system as it evolves from one state to the other.
Energy landscape: A mapping of all the possible configurations of a network and their associated energy.
It has to be noted that even when the geometrical/topological configu-ration of a network would allow the existence of folded states, such condi-tion is necessary but not sufficient for the network to actually reach them: the system might simply collapse into a jammed state. In order for the sys-tem to reach a folded state, its energy landscape must favour the correct folding path, that is, all the links need to deform in a precise sequence.
Luckily, the energy landscape itself can be tailored to such purpose, at least to some degree. Because buckling and bending both depend on the geometrical features of the links, changing those will affect the stress required to cause deformation; this implies that, if a steadily increasing stress is applied to a number of thin beams, the sequence in which they deform is determined by their geometries. Exploiting this simple tech-nique, one can effectively design the folding path of a network.
One last thing needs to be accounted for to have a complete picture of these processes: while, as we said, it is possible to tailor the energy land-scape in such a way that the system will naturally collapse in its folded states, nothing guarantees that such states exist in the first place. To date, we are not aware of any general rule that connects geometry and topology of a network to the presence of folded states. It has been noticed, how-ever, that one can organize groups of unit cells (e.g. small squares) into higher level structures that, up to a certain degree, move collectively; we will refer to those assuper-squares. If super-squares are tiled together in a pattern that is known to present a folded state, like that of the holey sheet, for instance, the network thus realized will also have such folded state. Moreover, if the super-square itself can fold into a folded state, than it is possible to design the energy landscape in such a way that both states will be sequentially visited, thus increasing the rank of the network.
This idea found an application in the work of van Hecke et al., in which a rank II structure was designed starting from the holey sheet. In this study, a super-square has been obtained by substituting to each squares of the holey sheet a group of five squares (see figure1.3a). Notice that this approach consists in substituting a rigid unit cell with a foldable one: the five-squares cross can fold onto itself, forming a smaller cross where the sides of the squares are in contact, instead of their vertices. The new net-work thus constructed presents two levels of unit cells, the squares and the crosses. As shown in figure1.3b, the crosses were tiled following the same pattern as the holey sheet. The connections between the crosses (red dots in figure1.3) were made much thinner than those connecting the squares within the crosses (green dots in figure1.3), so that they would buckle first; the super-squares thus fold once just like the holey sheet. When a folded
1.2 Physics of the experiment 5
state is reached (figure1.3d), the new pattern is again one that leads to a folded state, once the lower level unit cells (the individual squares) start moving: the network fully folds, reaching a compact configuration (figure
Figure 1.3:In a, b, c, d, e, f): Red dots represent connections that hinge during the first folding stages, green dots represent connections that hinge during the second folding stage. a) Two levels of unit cell: the five-diamonds cross is the upper level unit cell (super-square), each individual blue square is the lower level one. b) A design of the network used in the experiment of . Highlighted in blue are the squares forming the unit cells on the lowest level; in pink is shown the upper super-square, depicted as a bigger square to help recognize the holey sheet pattern it forms. c) Transition between unfolded network and first folded state. d) First folded state. e) Transition between the first and the second folded state. f) Second (and final) folded state of the HR II network.
1.2 Physics of the experiment 7
This experimental study revolves mainly around a single physical phe-nomenon, the buckling instability, which characterizes the behaviour of thin beams under axial compression. In fact, this phenomenon is what al-lows the folding processes to occur in the first place: the foldable network is a pattern of polygons formed by connecting them at their vertices with thin beams; under compression the beams buckle, causing the polygons to rotate and eventually get in contact with each other, and this is the folding process that we investigate in this research. We have restricted our study to patterns of either squares or triangles. What follows is a brief descrip-tion of the buckling instability.
Let us consider a beam of lengthLand cross-sectionab, and let us also consider a force F applied on ab along L. As long as F is smaller than a critical thresholdF < FB, the beam is deformed along the direction of the force; however, when F ≥ FB, a spontaneous symmetry breaking called buckling occurs, causing a displacement in a direction perpendicular to that of the force: the beam starts bending.
Figure 1.4: Buckling of a thin beam under uniaxial compres-sion along its length.
The threshold FB at which the insta-bility occurs depends on the geometrical features and the elastic properties of the beam, and can be calculated as:
FB = π 2EI
where: FB is the threshold force, E is the Young’s modulus of the beam, I is the area momentum of inertia of the cross sec-tion of the beam (I = a3b for a rectangu-lar section), L is the length of the beam .
Notably, an already bent beam is less stiff against further compression than a straight one; in other words, after the buckling instability has taken place, the
”chain” to be clamped to walls that can only move along the length of the beams. If the walls start compressing the chain with increasing pres-sure, the beams will buckle and then bend; if, however, the thicknesses of the different beams differ enough from each other (as expressed by equa-tion (1), the threshold force depends on the third power of the thickness, FB ∝ a3), it is possible that the strain required to buckle some links is not enough to deform others: some parts of the chain will deform consistently, while others will simply be displaced by the global motion, maintaining their shape essentially unaffected. In order for this to happen, a key role is played by symmetries: it can be observed during folding processes that some symmetries of the pattern, broken by the onset of buckling, are re-covered when self contact is reached. While the general reasons for this to happen are not yet understood, this occurrence is at the very base of our definition of multiple folding; in fact, in order to observe buckling (instead of bending) as a consequence of compression, the folded state needs to be such that the links in the network are symmetrically oriented against the stress: this way, the stress is equally applied to all the links along their (initial) axis.
Now that we have a clear picture of these processes, we ask a number of questions on their nature: can we isolate a single feature of a network that fully determines its foldability and rank? Is the construction rule that we have just presented for rank II networks general (can we apply it to other rank I patterns?) and is it possible to extend it in order to obtain networks with rank III?
In the following chapters we will give a brief description of the exper-imental apparatus and procedures adopted in this research, followed by an account of the different geometries we studied in order to investigate the questions mentioned above. We will then present in greater detail one particular pattern on which we focused, showing and explaining the re-sults we found when characterizing its response to biaxial compression. Finally, we will summarize our findings and outline possible directions that further studies on this subject may follow.
1.2 Physics of the experiment 9
Figure 2.1: Instron 5965 uniaxial testing device.
3D printer: All the networks used in this study have been directly printed using either a Lewihe Sneaker printer or a FELIX printer. Both printers work by extruding fused fila-ment from an electrically heated nozzle. The filament can be made of one of a selec-tion of materials: in this research we have used Filaflex, an thermoplastic elastomer fila-ment that allows for flexible prints. Its tech-nical specifications can be found in Appendix 2.
Mechanical testing: In order to exert stress on the printed networks, an Instron 5965 uniaxial testing device was used. This machine comprises of two clamps, one fixed at the bottom and the other on an upper section that can be moved ver-tically; the upper section also hosts a load cell that measures the forces exerted during the ex-periments. The machine can measure the vertical movement of the upper section with a resolution
12 Experimental realization
Figure 2.2:a) Uniaxial compression of a HR II network. b) Tulip-shaped clamps. Thanks to their geometry, they convert a uniaxial compression into a biaxial one.
Biaxial clamps: As it had been observed in previous studies , some geometries repond to uniaxial compression with all the beams buckling and bending in the same direction (see figure 2.2a), instead of the alter-nated pattern typical of folding structures. In order to obtain the desired behaviour, these networks need to be subjected to biaxial compression; however, the Instron 5965 can only compress uniaxially. To solve this prob-lem, a set of plexiglass tulip-shaped clamps, designed and built by LU Fine Mechanics department, was used to convert the uniaxial compression into a biaxial compression(figure2.2b).
Camera: All the experiments that have been conducted on our net-works have been video-recorded, acquiring images of the experiments via a Basler camera with a Tamron 28-300 lens at an aperture of 5.6 f-stops.
Lighting: During the tests the samples were illuminated by a combina-tion of frontal and rear lights, in order to provide enough light and contrast to acquire clear images. The rear illumination was given by a LED light panel (20x30 cm). The frontal illumination was provided by a neon lamp and two LED bike lights; all frontal lights needed to be placed at the sides of the apparatus, so as to avoid that reflections on the clamps affected the image acquiring.
2.1 Experimental apparatus 13
3D printing: For the design of the network, we have connected python scripting to FreeCAD, and exported .stl files; these files have successively been run through Cura, a software that translates them into a code that the printers could interpret and execute.
Data acquisition: Once the samples were implemented in the experi-mental apparatus (i.e. clamped in the Instron), we used a software called BluehillR to program and run the experiments. Image acquisition was controlled via a program developed in LabVIEW: this program connected the camera to the Instron, which would trigger snapshots at given times during the test, so that images and data could be synchronized. In typ-ical test, the sample would be first fully compressed by manually con-trolling the machine, in order to determine the total amount of vertical compression; this value would then be implemented in an automated test developed in BluehillR : the sample would be compressed with a rate of 5mm/s, with load and vertical displacement being measured every 100ms and pictures being acquired every 300ms with a resolution of 2048x2048 pixels, which corresponds to≈722.5x722.5 mm.
14 Experimental realization
We decided to track and analyse the motion of the unit cells during defor-mation, so that we could obtain more informations other than the mechan-ical response of the samples; in particular, we could investigate whether all symmetries of the system are broken between folded states. In order to detect the squares, we marked them with straight lines along their diago-nal; at first the marks were applied manually with a pen, in a later stage the lines were directly 3D printed on the network. Once the images were acquired, if the contrast between the marks and everything else was high enough, we could use ImageJ to threshold the images so as to keep only the marks; we could then fit ellipses on them, in such a way that the major axis of an ellipse would be aligned to the diagonal of a square; with this procedure, ImageJ provides position and orientation of the fitted ellipses (i.e. the marked squares) in every picture.
(a) (b) (c)
Figure 2.3: a) HR III network in the clamps. b) Thresholded image of a). c) Ellipses fitted on b).
2.1 Experimental apparatus 15
Because it is possible to associate with every picture a measurement of load/displacement coming from the Instron, the sequence of images also represents the time sequence of the experiment (every picture corresponds to a particular instant of the process). By having the data on the fitted el-lipses from every picture we were therefore able to effectively track posi-tion and orientaposi-tion of the squares throughout the whole process.
It has to be noted, however, that there are some important experimental difficulties with this procedure: if the contrast between marks and back-ground is not high enough during the whole process, at some time-step it can happen either that a mark is excluded from the picture (in which case the tracking algorithm stops following it), or that other parts of the sample become included in the picture and get treated as marks, affecting the shape and/or the number of the fitted ellipses. To address this prob-lem, we included the LED lights (to provide better illumination and, thus, better contrast) and we tilted the camera by 45o degrees (so as to align the sides of the picture frame with the side of the sample, thus effectively gaining a factor√2 in resolution).
16 Experimental realization
Calibration of the 3D printer
The main experimental limit of this study were given by the finite reso-lution of the camera, and by the precision and the quality the 3D printer could achieve. The final quality of the print would depend on a set of pa-rameters, such as the printing speed and each layer’s thickness, as well as it would vary with the overall size and complexity of the model.
In order to optimize the quality of the prints, the network in figure
2.5b has been printed several times; we could find the optimal settings for printing our patterns by comparing the quality of the resulting struc-tures (taking into account factors such as the accuracy in printing small parts, determined by measuring them and comparing them with the pro-grammed parameters, and the number and entity of eventual defects). The network (shown in figure2.5b) has been chosen as a good representation of the complexity that our prints required. From these tests, it turned out that the most influential settings were nozzle temperature, print speed and layer thickness; the optimal settings that we found can be seen in table2.1, while in Appendix 1 are reported the results for all the tests that we run.
A simpler print has instead been used to determine the maximum pre-cision the Sneaker could achieve: a number of ”dogbones” (two squares connected by a thin beam at the vertices) of different sizes were printed, showing that the machine could print parts as thin as 0.8 mm, with stan-dard deviation of±0.1 mm. It has to be noted, however, that the chance of printing failures (ranging from inaccuracies in the print to total clogging of the machine) would increase considerably with the size of the network and its complexity. In the final stages of the present study, where accuracy would be crucial for the experiments, these issues resulted to be too im-pairing, and some networks have been built with the FELIX printer by J. Mesman-Vergeer from the Fine Mechanics department of L.U.
2.1 Experimental apparatus 17
Sneaker’s basic parameters (unchanged during all tests):
Layer height 0.2 mm Nozzle size 0.4 mm
Shell thickness 0.4 mm Retraction speed 40 mm/s
Bottom-top thickness 0.4 mm Retraction 4.5 mm
Fill density 100% Z-hop when retracting 0.075 mm
Sneaker’s optimal settings:
Printing speed 35 mm/s Temperature 230 C
Minimum travel for retraction 5 mm Skirt lines count 2
Table 2.1:Optimal settings found during the calibration of the Sneaker 3D printer.
Figure 2.5:a) A chain of ”dog-bone” structures used to determine the maximum accuracy of the Sneaker printer. The diagonal of the squares is≈ 4mmlong and the thicknesses of the connections, from thickest to thin, are ≈ 2mm, ≈ 0.8mm,
18 Experimental realization
At the beginning of this research, there were two very broad questions: why do some networks fold while other don’t, and is it possible to build a network that shows three sequential folded states? What follows is an account of the different strategies we have tried in order to answer the sec-ond question, some successful and some not, while expanding our knowl-edge to answer the first.
Figure 2.6: Three hi-erarchies of unit cell; the super-square II is marked in yellow, the super-square I in red and the lowest level unit cell (the last one to ro-tate) in light blue.
A first attempt at building a rank III model con-sisted in extending the hierarchical construction; the network showed in figure2.7ais the resulting model. As it can be seen in the picture, the hierar-chical approach was (mistakenly) applied only to the central section of the network (compare with figures 2.6 and 2.7b), forming a less symmetric pattern on the super-square II. This inevitably re-sulted in the disruption of the expected folded state -the network would always jam under biax-ial compression (see figure2.7d).
While this model represented a failure in the attempt of creating a rank III structure, it still proved to be instructive, as it highlighted the strong influence of the boundaries of the struc-tures on their folding processes.
A second model, depicted in figure 2.7c, was used to investigate the possibility of changing the size of some squares to favour their rotation. The
resulting network indeed proved to be of rank II, as expected (two differ-ent sizes of squares, equivaldiffer-ent of the 2 differdiffer-ent thicknesses in the regular rank II network), without the need to vary the thickness of any link. The extension of this approach to a rank III network, however, was discarded, despite it being theoretically sound; this is because it required squares of three exponentially increasing sizes, thus exceeding either the maximum printable surface allowed by the Sneaker, or its accuracy in printing small parts.
2.2 Exploration phase 19
(a) (b) (c)
20 Experimental realization
2.2 Exploration phase 21
Figure 2.8: Folding steps of a windmill network.
In parallel with the experiments on networks with square-shaped unit cells, other geometries were being tested.
In particular, we designed a unit cell consist-ing of a network of rectangles of increasconsist-ing size (see figure 2.8) extending from a central square. The idea behind this design was to build a system which could fold from the center outwards, with the rectangles connected to the central square col-lapsing at its sides, forming a bigger square; at ev-ery folding step, the central square would become bigger, while the arms extending from its vertices would become shorter, until full closure. Such a unit cell could then be tiled, for instance with a holey sheet pattern, to build a network of any de-sired rank.
When experimentally realized, this unit cell proved to work as designed only partially: the system would collapse under compression as ex-pected, but there would be only one onset of buck-ling instabilities, followed by continuous bend-ing until full closure; these system proved there-fore not to be sequential in their shape-changing. Moreover, all experimental realizations of tiling were met with failure: the links would never buckle and bend in the correct sequence, leading instead to a jammed state. While this could simply be the result of not enough accuracy in designing the energy landscape for the system, we decided
not to insist on this particular design, and instead focused on the hierar-chical rank 3 squares network.
22 Experimental realization
Figure 2.9: Cuts in a square can allow it to unfold into triangles .
One other approach used to design a rank 3 net-work was inspired by the net-work of Ron Resch . From his work we took the idea of making cuts in regular polygons to open them into rings of trian-gles. In particular, there is a way (see figure2.9) to make a square unfold into four connected tri-angles.
Our first idea has been to apply this technique to the rank II model (see figure2.10a): upon com-pression, the network would first fold into the rank II configuration, and then behave regularly, folding two more times; the system would then be of rank III in total. While it was a sound model in theory, experimentally it proved to be too
chal-lenging to print accurately, thus leading only to partial success (only the first folding stage would occur as programmed). We decided not to inves-tigate further in this direction, as even if it could work, it would not teach us much about the physics of folding processes.
A second application of the ”unfolding polygons” approach consisted in a holey sheet-like tiling of 4-fold split squares (see figure 2.10b and
2.10c). The network thus created showed a set of remarkable properties: It is compliant to uniaxial compression from both directions.
In both directions it behaves as a rank 2 network, without the need to differentiate the thickness of the links to separate their deformation in time.
Even when fully folded, some of the unit cells at the boundaries would be free to move.
This network provided us with an important insight on these processes: in fact, while being topologically and geometrically different from the rank II model of the previous study, it would still present a two-steps folding behaviour. Moreover, for this network, the key role is played by geometry and self contact, as they seem to guarantee the correct folding path.
2.2 Exploration phase 23
24 Experimental realization
Focus: the hierarchical approach
As already announced in the previous sections, at the end of the explo-ration phase we decided to focus on the hierarchical approach only: is it possible to use it to obtain networks of rank III or higher? If so, how and why does it work?
In order to extend the hierarchical approach to rank III, one has to re-peat the same procedure (substituting every square with a group of five) to the HR II network. Intuitively, the network will have a greater number of links that can bend, and will thus have more possibilities to end up in a jammed state; this happens because any link that deforms at the wrong time-step causes the displacement of at least two squares, breaking the symmetric pattern of the folded state and causing an extra stress on the neighbouring connections, which, in turn, will be more likely to deform at the wrong time.
However, it is an easy mental exercise to find the folding path that leads to three folded states: one has to start with the super squares II and recognize that they are set in the same pattern as a holey sheet, thus they can fold following the same motions; once self contact is reached, a new level of unit cells can be defined, following the same pattern as the HR II first folded state, and it is then possible for the system to fold again. When a new folded state is reached, the lowest level unit cells (the individual squares) are again in the same pattern as the super-squares in the previ-ous state, thus they can fold once more, leading to full self contact. Figure
2.11 shows the folding steps and different levels of unit cells of this pro-cess.
One can then realize that there must be 3 sets of links deforming at differ-ent times. In order to obtain this behaviour, it follows that there will have to be links of three different thicknesses, in order for the energy landscape to favour the correct folding path; a limit case would be for all the links to have the same thickness, which proved to work for the HR II network.
While this approach seems sound in theory, the first experimental real-izations of the network all led to failure; not only using links all of the same thickness would always result in a jammed state, but even assigning different thicknesses to the connecting beams (following the hierarchical procedure) didn’t produce the expected folded states: the network would often reach the first folded state, but then small imperfections would make it deviate into a jammed state.
What follows is an account of all the aspects of this experiment that could disrupt the correct folding process.
2.3 Focus: the hierarchical approach 25
Figure 2.11: a, b, c) Red dots: first connections to buckle; green dots: second connections to buckle; blue dots:connections that will buckle last. a) Unfolded HR III network. b) First folded state of the HR III network. c) Second folded state of the HR III network. d) Final folded state.
First of all, we observed that when there is only a small difference between the thickness of the three sets of links, some of the connections bend before their due time, deforming the network and preventing it from reaching the folded states.
In order to correct this behaviour, a high contrast in the thicknesses of the links is required. However, the printable surface is fixed (for the Sneaker, the maximum printing area is ≈ 300x185mm), thus limiting the maximum size of the network; moreover, it has been shown  that the capability of a network to fold depends also on its porosity, a parame-ter that describes the size of the holes compared to the overall size of the network; by directly printing networks with the geometry of the second folded state (figure2.11c) and compressing them, we found that the thick-est connections need to be less than 12 the diagonal of the squares in order for the network to fold. Finally, the thinnest parts that can be printed by the Sneaker are about double the nozzle size, thus ranging around 0.8-0.9 mm. There was therefore a strict experimental limit to the maximum contrast we could realize in the thicknesses of our printed networks(the thinnest part being≈0.4 times as thick as the thickest).
specifica-26 Experimental realization
tions of the links in order for the correct sequence of folding to take place. As it can be seen from table 2.2, doubling the thickness of a connection would not produce an increase in the buckling load of a factor 8, as one would expect from the theory (FB ∝ a3); this is because, by increasing the thickness of the beam connecting two squares, one increases also its length by the same amount (compare figures 2.12a and 2.12c). We con-cluded that, given all this limitations, we would need to differentiate not only the thickness of the links, but also their height (upon which the buck-ling stress depends linearly).
Buckling load tests on ”dog-bones” Thickness(mm): Buckling Load (N):
Table 2.2:Stress required to buckle connections of different thicknesses.
(a) (b) (c)
Figure 2.12: Three ”Dog-bones” used to optimize the contrast between links of different hierarchies. a) Thickness:1.6mm. b)1.2mm. c)0.8mm.
One other factor that we found to play against the folding process is friction, which opposes to the motion of the squares. If the surface of the clamps and/or that of the squares themselves are not uniform, some of the squares might be more obstructed than others in their motion, resulting in an asymmetric global deformation that ends in a jammed state. As we will explain in greater detail later, this is particularly true for the squares at the boundaries.
2.3 Focus: the hierarchical approach 27
Finally, it has to be noted that the printed networks are not fully elastic: after the first compression, they revert to a slightly deformed state; this is-sue is enhanced by the fact that the networks are held in a vertical position when compressed, and are thus further deformed by the pull of gravity. Because of that, the initial buckling instability and the consequent sym-metry breaking are not observed after the first compression. The choice of vertical positioning, however, was justified by the consequently reduced friction against the plates of the clamps.
28 Experimental realization
As already observed in the previous sections, the boundaries of the net-work play a determining role in the folding process. Boundary squares undergo greater friction, compared to the bulk ones, as they are in con-tact with the compressing surface; moreover, because of the shape of the clamps (interlaced plexiglass panels, with enough space between panels for them to slide between each other), it is possible for the squares to de-form and become partially stuck between plates, further impeding their correct motion; finally, after the first folded state, the corner squares end up having two sides in full contact with the sides of the clamps, and are often prevented from further rotation.
During the experiments, we have observed that such imperfections at the boundaries often propagate to the bulk of the network as the stress is increased (see figure 2.14. We decided not to study this diffusion of ”defects”(mis-steps in the correct folding sequence), but we concluded that at least 9 super-squares are required (8 at the boundaries plus a central one) to have at least the central section of the network folding correctly.
Figure 2.14: From top left to bottom right: propagation of ”defects” from the boundaries to the bulk during the folding process.
Rank III folding
After calibrating and optimizing the design of the network, we found a successfully folding network characterized by thicknesses as reported in the following table:
Figure 3.1 shows a plot of the force applied as a function of the strain (vertical displacement divided by total length in open configuration). As explained in the theory section, the force required to buckle a beam is con-siderably greater than that required to bend it; as a consequence, in a plot of force against strain, one expects the curve to be steep before a buckling instability takes place, and relatively flat afterwards; if multiple buckling instabilities occur at different moments, the resulting plot should appear step-like.
In our case, we expect three flat regions in the plot, representing the bending phase that follows a buckling instability, separated by the steep increases characteristic of buckling. Indeed, we can observe in the graph that the blue curve behaves as we would expect from the theory, excep-tion made for the missing initial steep jump corresponding to the initial
Hierarchy level III Hierarchy level II Hierarchy level I
a (mm) 0.9 1.2 1.6
L (mm) 0.9 1.2 1.6
b (mm) 3.5 10 10
buckling instability: as anticipated, this is due to the imperfect elasticity of the network that, combined with the gravity pull, deform the initial state breaking its symmetry. One other notable feature of this plot is the increasing steepness of the curve: this effect is caused by the increasing number of links that need to buckle at every successive folding step. The system therefore alternates states of compliance to stress with states of in-creasing stiffness.
Figure 3.1:Force plotted as function of the strain. In blue, an HR III network with the geometries specified in table3.1; in red, an equilink HR III network.
The red curve shows instead the same plot for a network in which all the links have the same dimensions, to which we will refer asequilinkfrom now on. The smooth shape of the curve shows a disordered deformation of the links, and it keeps on increasing as more squares reach self contact, preventing their links to bend further and deforming through compres-sion instead. In the final stages of comprescompres-sion, however, we can notice that the load required to further compress the equilink is actually lower
3.1 Rank III folding 31
than that for the other network; this means that it hasn’t reached a fully closed configuration when the correctly folding network, represented by the blue curve, is in its final state. A comparison between the two curves shows the striking effectiveness of the approach used to tailor the energy landscape of the system: by a small variation in the geometrical parame-ters of the network, one can greatly vary the mechanical response of the system to biaxial stress.
Figure 3.2: a, b, c, d)Colored areas represent different stages of the folding pro-cess; yellow areas show when the network is in a folded state, and green areas highlight the region in which it has reached the final, fully folded state. a) Load as a function of strain in a holey sheet (HR I) network. b) Load as a function of strain for an equilink HR II network. c) Load as a function of strain for a HR III network. d) Load as a function of strain for an HR III equilink network.
3.2 Rotations and symmetries 33
Rotations and symmetries
Another quantity that we can use to characterize these multi-step fold-ing processes is the relative orientation of the squares: after bucklfold-ing, the beam connecting two squares bends, thus the angle between the two unit cells transits from 0 (straight beam) to π
2 (self contact reached).
For a plot ofθ(the relative orientation of two adiacent squares) against strain in an HR III, which is shown in figure3.3c, it is to be expected that all links will follow one of three curves (or their symmetric correspondents at negative angles), all with the same shape, but each one starting at a different strain, corresponding to the onset of a set of buckling instabilities. To be more precise, one should expect one curve to start deviating from constant 0 when the previous curve reaches π
2; this, in fact, translates into the new set of connections buckling after the previous set has reached self contact.
Conversely, in an equilink network (shown in figure 3.3d), it is to be expected that the relative orientations of all links will start to vary at ran-dom moments, and will follow a less sharp transition, not always ending up atθ=π/2, as the system jams into a disordered state.
By studying figure3.3c, we can see that our networks behave in good agreement with our theoretical expectations described above. We can also observe, however, the experimental limits of this study: not all curves start from θ = 0, showing that the networks are already partially bent; more-over, the bending of different links of a same hierarchy don’t always fol-low the same path, with some reaching π/2 earlier than others or not at all, which means that the deformation is not simultaneous throughout the whole network. It has to be noted, however, that while this could be be-cause of imperfections in the network, it could also be an artifact be-caused by insufficient precision in the detection of the marks: shadows or partially bent lines (for instance, due to deformation of the squares) could alter the shape of the fitted ellipses, altering their extrapolated angle.
its connections being all of the same thickness, while in the HR III a strong geometrical differentiation between the hierarchies had to be introduced to obtain the expected behaviour. We believe the behaviour of the HR II network to be a limit case, allowed by its particular topology (only unit cells with either four or two vertices connected, apart from the bound-aries). Finally, it should be noted that the bending angle of the thinnest connections in HR I and HR II networks averages to 0. This is due to an extra symmetry inherent to the folding of the holey sheet pattern (which all unit cells of the highest hierarchical level follow): as was shown in fig-ure1.1, adiacent unit cells of a holey sheet rotate in opposite directions (i.e. the bending angles of two consecutive connections have opposite signs); this is not the case for the links of the other hierarchies, which all bend in the same direction. It can be seen in figure3.3c that the bending angle of connections belonging to the first hierarchical level would appear to break this symmetry; this result, however, is just a consequence of the limited number of such connections being tracked: because only one entire super-square II could be printed, there were not any two adiacent connections of the first hierarchy to track.
3.2 Rotations and symmetries 35
We have already noticed that the system doesn’t fully fold unless the con-trast between the links is high enough. We have decided then to study how the order of the system (how ”well” the network folds) changes at different contrasts.
Figure 3.4:Example ofθj.
In order to do so, we first need to de-fine a quantity that describes the ge-ometry of the beams. It seems nat-ural to borrow it from the equation that regulates the buckling load, so we will define the geometrical factor Gi ≡ a3ibi/L2i; we can then define the con-trast between two links i,j as Ci,j ≡ Gi/Gj.
Now, we need a more precise definition of ”order” for our systems. As we know,
the final state of a fully foldable network is that in which all holes are closed. We can then refer to the state as ordered if this is true, and define it instead more or less disordered when there are holes that cannot be closed without deforming the squares themselves. In the case of the HR III net-works in study, when the final state is ordered all the squares are arranged into a square lattice. We can then formally quantify the order of the sys-tem by introducing anorder parameterψthat describes the deviation of the system from the ideal configuration.
Let us now give a formal definition of ψ. Let Γ be the center of a square, and let ˆxbe an arbitrary axis (for instance, a horizontal axis) pass-ing throughΓ. Let then jbe a neighbour ofΓat (polar) coordinates(rj,θj), where the angle is measured in relation to ˆx. We can then define:
ψ= 1 N
where N is the total number of squares considered, Nj(Γ) is the number of neighbours of each Γ, and m is an integer that normalizes ψ to one when the system is ordered; for instance, for an ideal square lattice, all neighbours are positioned at θ = 0, π, and ±π/2, thus m = 4n (with n=1, 2, 3, ... integer) leads toψ=1.
The concept of ”neighbour”, however, can be elusive if referred to a jamming, disordered network; in practical terms, it is difficult to
3.3 Order parameter 37
mine from an image whether two square should be considered as neigh-bouring or not. To dissipate this ambiguity, we make use of the Voronoi tessellation with Euclidean distance. Let us consider any set of N points (referred to asseeds) in a plane; the plane can then be partitioned inNcells, each containing all the points that are closer to one particular seed than to any of the others. In our case, we can identify the position of the center of each square with a seed of a Voronoi cell, in which the distance of a point to the seed is calculated according to Euclidean metric. We can then define two squares as neighbours if their Voronoi cells are neighbouring.
Figure 3.5: Voronoi tessellation of the central section of an HR III network in its first folded state.
Figure 3.6: Tracked positions of the squares of a unit cell of highest level, at dif-ferent strains, corresponding to the folded state of a HR III network; highlighted are the Voronoi cells generated around each square, color coded (from dark red to dark blue) to represent their local contribution toψ.
Figure3.7 shows the plot ofψagainst strain for the folding process of four networks with different hierarchies: HR I, HR II, an HR III character-ized byC1 = 1.5,C2 = 3.8 (a fully folding network), and an equilink HR III. As we can see, the rank I network starts as fully ordered, coherently with our definition of order; during the deformation, the order decreases due to the boundary frustrations discussed in the previous paragraph. The order of the networks with HR II and HR III shows sharp peaks in spondence to the reaching of a folded state, followed by steep drops corre-sponding to the symmetry breaking caused by buckling; it has to be noted that both networks show, on average, a relatively low order (≈0.5): this is to be attributed to a number of experimental causes, mainly imperfections in the detection and tracking of the squares (which affects the estimated position of the seeds of the voronoi cells), and limited number of squares tracked (resulting in empty areas in the final folded states). Moreover, the order of the HR III networks appears to be higher at the end of the process; however, this is a result of the initial pre-bent state, in which the system is less ordered than in its ideal open configuration. Finally, we can see that the order of the equilink network decreases during the whole process, compatibly to its jamming path, with some oscillations caused by parts of the network reaching self-contact and forming temporarily or-dered islands.
By looking at the values of strain at which the networks reach their folded states (highlighted by the peaks in the value of the order parame-ter), we can see that they are in good agreement with what would be ex-pected from geometrical considerations: in correspondence to the folded states, the strain should assume values of 1− 1
(√2)m, wherenis the
hierar-chy of the folded state (e.g. n = 1 for the first folded state, n = 2 for the second folded state, and so on). A small discrepancy from these values for the HR III networks is explained again by its initial pre-bent configuration,
3.3 Order parameter 39
which was considered the starting point of the test (at which the strain was set=0); while this affects the quantitative precision of the measurements, it leaves unaffected the qualitative validity of our results.
Figure 3.7: a) Plot ofψagainst strain for an HR I network; the inset shows the
voronoi tessellation of the tracked portion network at different values of strain. b) Plot ofψagainst strain for an HR II network; the inset shows the voronoi
tes-sellation of the folded states of the network. c) Plot ofψagainst strain for an HR
III network withC1 = 1.5,C2 = 3.8; the inset shows the voronoi tessellation of the folded states of the network. d) Plot of ψagainst strain for an HR III
Summarizing, in this study we have built a number of foldable network of various ranks, proving the effectiveness of direct 3D print and, at the same time, expanding the general knowledge on the folding processes.
First of all, we have found that the energy landscape of the system plays a fundamental role in the process, as folded states can be reached only if the correct folding path is is favoured. This implies that the ”fold-ability” of a network is not intrinsic to its topology. Moreover, we have also found that the energy landscape for this networks depends almost entirely on very few parameters, such as the thickness of the beams, and is therefore easily tunable.
We have also found that different geometries can be combined in dif-ferent hierarchical levels, augmenting the total rank of a network. This simple fact widens greatly the number of options for designing networks with preprogrammed responses, allowing for a more precise tailoring of material properties and the development of a class of materials sensitive to their environment.
Focusing on these networks, we have studied experimentally their me-chanical response, finding it in good agreement with theoretical predic-tions, within the experimental limits. Moreover, we have tracked the mo-tion of the single squares and confirmed again the expected behaviour. From our data, we can conclude that in hierarchical networks the folding process can be subdivided in separate stages, in each of which the be-haviour of the network is entirely regulated by a single hierarchy. In other words, in a HRnnetwork, the mechanical response is first determined by the links belonging to hierarchy n(i.e. the links connecting the unit cells of the highest level); once the first set of squares reaches self contact, these connections stop playing a role, and the response is further determined only by the links of hierarchyn−1, until they too reach self contact, and so on.
Finally, we have fully characterized the order of these systems with a single parameter, and we have studied its evolution throughout the fold-ing process of four hierarchical networks that follow different foldfold-ing paths. We found that the order increases when the system evolves towards a folded configuration, reaching a local maximum in correspondence of self-contact, and it drops steeply during a new onset of buckling instabilities; conversely, the order of the system decreases steadily when the folding path leads to a jammed state.
Our research could lead to a number of applications, from deployable technologies that can be folded during transportation and become opera-tional once unfolded, to complex electronic parts (exploiting self contact to create different circuits at different folding states), to soft robotic parts that can dynamically change their compliance to external stresses by rear-ranging into folded states.
A number of questions however remain still open: would it be possible to engineer the energy landscape of hierarchical networks so that they fold starting from the lowest level unit cell up? If it is not possible, is there a fundamental reason for that? When a folding step is imperfect (compared to the ideal path that leads to a folded state), how does this mis-step prop-agate during the process? How does the order of the network depends on the contrasts between the connections, and how does this change with the rank of the network? More in general, is it possible to extend these findings to 3D materials? Are there other ways to actuate the folding pro-cess, other than mechanical compression? Is there a generic rule to design materials that can fold in 2 or 3 dimensions?
There is still a lot of space for research in this field, which could
Quality tests for different settings:
Sneaker’s Settings Test # 1:
Printing speed 50 mm/s Temperature 230 C
Minimum travel for retraction 5 mm Skirt lines count 1 Results:
Not a high quality print, many loose/stray filaments, imperfections in the squares.
Sneaker’s Settings Test # 2:
Printing speed 50 mm/s Temperature 230 C
Minimum travel for retraction 5 mm Skirt lines count 2 Results:
Same as test # 1, but with less mistakes in the initial layer.
Sneaker’s Settings Test # 3:
Printing speed 35 mm/s Temperature 230 C
Minimum travel for retraction 5 mm Skirt lines count 2 Results:
Reasonably high quality, well-shaped squares and few stray filaments.
Sneaker’s Settings Test # 4:
Printing speed 35 mm/s Temperature 230 C
Minimum travel for retraction 2 mm Skirt lines count 2 Results:
46 Appendix 1
Sneaker’s Settings Test # 5:
Printing speed 35 mm/s Temperature 220 C
Minimum travel for retraction 5 mm Skirt lines count 2 Results:
Almost no stray filaments, well-shaped squares, mistakes in the first layers.
Sneaker’s Settings Test # 6:
Printing speed 35 mm/s Temperature 240 C
Minimum travel for retraction 5 mm Skirt lines count 2 Results:
Bad quality print, many stray filaments and extra connections between the squares.
Filaflex technical specifications:
Diameter 1.75 mm
Printing speed 30−50mm/s Printing temperature 230−250C◦
Shore hardness (A) 84
Tensile strength 39
 Schittny R., Buckmann T., Kadic M., and Wegener M. Elastic measure-ments on macroscopic three-dimensional pentamode metamaterials. Appl. Phys. Lett., 103(231905), 2013.
 T. Buckmann, M. Thiel, M. Kadic, R. Schittny, and M. Wegener. An elasto-mechanical unfeelability cloak made of pentamode metamate-rials. Nature Communications, 5(4130), 2014.
 B. Florijn, C. Coulais, and M. v. Hecke. Programmable mechanical metamaterials. Phys. Rev. Lett., 113(175503), 2014.
 R. Oftadeh, B. Haghpanah, D. Vella, A. Boudaoud, and A. Vaziri. Optimal fractal-like hierarchical honeycombs. Phys. Rev. Lett., 113(104301), 2014.
 C. Coulais, J. T. B. Overvelde, L. A. Lubbers, K. Bertoldi, and M. v. Hecke. Discontinuous buckling of wide beams and metabeams. Phys. Rev. Lett., 115(044301), 2015.
 B.I. Popa, L. Zigoneanu, and S. A. Cummer. Experimental acoustic ground cloak in air. Phys. Rev. Lett., 106(253901), 2011.
 T. Mullin, S. Deschanel, K. Bertoldi, and M. C. Boyce. Pattern trans-formation triggered by detrans-formation.Phys. Rev. Lett., 99(084301), 2007.
 Fr´e Vink. Multiple shape changes in mechanical metamaterials. Bsc. thesis, Leiden University, 2015.
 Z. P. Baˇzant and L. Cedolin. Stability of Structures: Elastic, Inelastic, Fracture, and Damage Theories. Courier Corporation, 1991.
 R. Resch. The ron resch paper and stick movie. 1992.
 Bertoldi K., Reis P. M., Willshaw S., and Mullin T. Negative pois-son’s ratio behavior induced by an elastic instability. Adv. Matter., 22(361–366), 2010.